# this file is part of refractiveindex.info database
# refractiveindex.info database is in the public domain
# copyright and related rights waived via CC0 1.0

REFERENCES: "<a href=\"http://refractiveindex.info/download/data/2017/schott_2017-01-20b.agf\">SCHOTT Zemax catalog 2017-01-20b</a> (obtained from <a href=\"http://www.schott.com/advanced_optics/english/download/\">http://www.schott.com</a>)<br>See also <a href=\"http://refractiveindex.info/download/data/2017/schott_2017-01-20.pdf\">SCHOTT glass data sheets</a>"
COMMENTS: "lead containing glass type        "
DATA:
  - type: formula 2 
    wavelength_range: 0.35 2.5
    coefficients: 0 1.46141885 0.0111826126 0.247713019 0.0508594669 0.949995832 112.041888
  - type: tabulated k
    data: |
        0.350 1.3048E-06
        0.365 3.6564E-07
        0.370 2.6281E-07
        0.380 1.5462E-07
        0.390 1.0351E-07
        0.400 6.5309E-08
        0.405 5.3969E-08
        0.420 3.6593E-08
        0.436 2.5209E-08
        0.460 1.7677E-08
        0.500 1.1180E-08
        0.546 6.9658E-09
        0.580 7.3996E-09
        0.620 9.8924E-09
        0.660 1.0531E-08
        0.700 8.9305E-09
        1.060 1.3523E-08
        1.530 6.3727E-08
        1.970 6.6068E-07
        2.325 2.2284E-06
        2.500 3.3066E-06
SPECS:
    n_absolute: false
    wavelength_vacuum: false
    temperature: 20.0 °C
    thermal_dispersion:
      - type: "Schott formula"
        coefficients: 2.59e-06 1.76e-08 -2.03e-11 1.17e-06 1.09e-09 0.255
    nd: 1.6727
    Vd: 32.21
    glass_code: 673322.407
    glass_status: standard
    density: 4.07 g/cm<sup>3</sup>
    thermal_expansion:
      - temperature_range: -30 70 °C
        coefficient: 8.2e-06 K<sup>-1</sup>
      - temperature_range: 20 300 °C
        coefficient: 9e-06 K<sup>-1</sup>
    dPgF: 0.0023
    climatic_resistance: 1.0
    stain_resistance: 1.0
    acid_resistance: 2.0
    alkali_resistance: 2.3
    phosphate_resistance: 3.0
